Passive Q-switch laser operation of circular , buried depressed-cladding waveguides realized by direct fs-laser beam writing in Nd : YAG / Cr 4 + : YAG composite media

Circular, buried depressed-cladding waveguides were inscribed by direct fs-laser beam writing in diffusion-bonded Nd:YAG/Cr:YAG composite media. Passive Q-switch operation was achieved using the pump at 807 nm with a fiber-coupled diode laser. Laser pulses at 1.06 μm with energy of 15.7 μJ and 3.9-ns duration (corresponding to a peak power of 4.0 kW) were obtained from a waveguide of 150-μm diameter that was realized in a 10.3mm long, 1.0-at.% Nd:YAG/Cr:YAG composite medium. The length of Nd:YAG crystal was 7.0 mm and initial transmission of Cr:YAG saturable absorber crystal was 0.70. The average output power reached 1.13 W. © 2017 Optical Society of America OCIS codes: (140.3580) Lasers, solid-state; (140.3530) Lasers, neodymium; (140.3540) Lasers, Q-switched; (230.7380) Waveguides, channeled; (130.3990) Micro-optical devices. References and links 1. C. Grivas, “Optically pumped planar waveguide lasers, Part I: Fundamentals and fabrication techniques,” Prog. Quantum Electron. 35(6), 159–239 (2011). 2. C. Grivas, “Optically pumped planar waveguide lasers, Part II: Gain media, laser systems, and applications,” Prog. Quantum Electron. 45–46, 3–160 (2016). 3. K. M. Davis, K. Miura, N. Sugimoto, and K. Hirao, “Writing waveguides in glass with a femtosecond laser,” Opt. Lett. 21(21), 1729–1731 (1996). 4. A. Ródenas, G. A. Torchia, G. Lifante, E. Cantelar, J. Lamela, F. Jaque, L. Roso, and D. Jaque, “Refractive index change mechanisms in femtosecond laser written ceramic Nd:YAG waveguides: micro-spectroscopy experiments and beam propagation calculations,” Appl. Phys. B 95(1), 85–96 (2009). 5. T. Calmano, J. Siebenmorgen, O. Hellmig, K. Petermann, and G. Huber, “Nd:YAG waveguide laser with 1.3 W output power, fabricated by direct femtosecond laser writing,” Appl. Phys. B 100(1), 131–135 (2010). 6. J. Siebenmorgen, T. Calmano, K. Petermann, and G. Huber, “Highly efficient Yb:YAG channel waveguide laser written with a femtosecond-laser,” Opt. Express 18(15), 16035–16041 (2010). 7. Y. Tan, A. Rodenas, F. Chen, R. R. Thomson, A. K. Kar, D. Jaque, and Q. Lu, “70% slope efficiency from an ultrafast laser-written Nd:GdVO4 channel waveguide laser,” Opt. Express 18(24), 24994–24999 (2010). 8. A. G. Okhrimchuk, A. V. Shestakov, I. Khrushchev, and J. Mitchell, “Depressed cladding, buried waveguide laser formed in a YAG:Nd crystal by femtosecond laser writing,” Opt. Lett. 30(17), 2248–2250 (2005). 9. A. Okhrimchuk, V. Mezentsev, A. Shestakov, and I. Bennion, “Low loss depressed cladding waveguide inscribed in YAG:Nd single crystal by femtosecond laser pulses,” Opt. Express 20(4), 3832–3843 (2012). 10. H. Liu, Y. Jia, J. R. Vázquez de Aldana, D. Jaque, and F. Chen, “Femtosecond laser inscribed cladding waveguides in Nd:YAG ceramics: fabrication, fluorescence imaging and laser performance,” Opt. Express 20(17), 18620–18629 (2012). 11. N. Pavel, G. Salamu, F. Jipa, and M. Zamfirescu, “Diode-laser pumping into the emitting level for efficient lasing of depressed cladding waveguides realized in Nd:YVO4 by the direct femtosecond-laser writing technique,” Opt. Express 22(19), 23057–23065 (2014). 12. Y. Ren, G. Brown, A. Ródenas, S. Beecher, F. Chen, and A. K. Kar, “Mid-infrared waveguide lasers in rareearth-doped YAG,” Opt. Lett. 37(16), 3339–3341 (2012). 13. S. Müller, T. Calmano, P. Metz, N.-O. Hansen, C. Kränkel, and G. Huber, “Femtosecond-laser-written diodepumped Pr:LiYF4 waveguide laser,” Opt. Lett. 37(24), 5223–5225 (2012). Vol. 7, No. 7 | 1 Jul 2017 | OPTICAL MATERIALS EXPRESS 2496 #293432 https://doi.org/10.1364/OME.7.002496 Journal © 2017 Received 26 Apr 2017; revised 8 Jun 2017; accepted 8 Jun 2017; published 20 Jun 2017 14. F. Chen and J. R. Vázquez de Aldana, “Optical waveguides in crystalline dielectric materials produced by femtosecond-laser micromachining,” Laser Photonics Rev. 8(2), 251–275 (2014). 15. D. Choudhury, J. R. Macdonald, and A. K. Kar, “Ultrafast laser inscription: perspectives on future integrated applications,” Laser Photonics Rev. 8(6), 827–846 (2014). 16. G. Salamu, F. Jipa, M. Zamfirescu, and N. Pavel, “Cladding waveguides realized in Nd:YAG ceramic by direct femtosecond-laser writing with a helical movement technique,” Opt. Mater. Express 4(4), 790–797 (2014). 17. G. Salamu, F. Jipa, M. Zamfirescu, and N. Pavel, “Watt-Level Output Power Operation from Diode-Laser Pumped Circular Buried Depressed-Cladding Waveguides Inscribed in Nd:YAG by Direct Femtosecond-Laser Writing,” IEEE Photonics J. 8(1), 1500209 (2016). 18. G. Salamu and N. Pavel, “Power scaling from buried depressed-cladding waveguides realized in Nd:YVO4 by femtosecond-laser beam writing,” Opt. Laser Technol. 84, 149–154 (2016). 19. Y. Jia, C. Cheng, J. R. Vázquez de Aldana, G. R. Castillo, B. R. Rabes, Y. Tan, D. Jaque, and F. Chen, “Monolithic crystalline cladding microstructures for efficient light guiding and beam manipulation in passive and active regimes,” Sci. Rep. 4(1), 5988 (2014). 20. W. Nie, Y. Jia, J. R. Vázquez de Aldana, and F. Chen, “Efficient second harmonic generation in 3D nonlinear optical-lattice-like cladding waveguide splitters by femtosecond laser inscription,” Sci. Rep. 6(1), 22310 (2016). 21. A. Okhrimchuk, “Femtosecond fabrication of waveguides in ion-doped laser crystals,” in Coherence and Ultrashort Pulse Laser Emission, Dr. F. J. Duarte, ed. (Intech, 2010). http://www.intechopen.com/books/coherence-and-ultrashort-pulse-laser-emission/femtosecond-fabrication-ofwaveguides-in-ion-doped-laser-crystals. 22. T. Calmano, A.-G. Paschke, S. Müller, C. Kränkel, and G. Huber, “Q-Switched operation of a fs-laser written Nd:YAG/Cr:YAG monolithic waveguide laser,“ in Lasers, Sources, and Related Photonic Devices, OSA Technical Digest (CD) (Optical Society of America, 2012), paper IF2A.4. 23. T. Calmano, S. Müller, C. Kränkel, and G. Huber, “Multi-Watt Continuous Wave Output Power and Q-switched Laser Operation of Femtosecond-Laser Inscribed Yb:YAG Based Waveguides,“ 6th EPS-QEOD Europhoton Conference, Solid State, Fibre, and Waveguide Coherent Light Sources, 24-29 August, 2014, Neuchâtel, Switzerland, presentation WeD-T2-O-05. 24. Y. Tan, Q. Luan, F. Liu, F. Chen, and J. R. Vázquez de Aldana, “Q-switched pulse laser generation from doublecladding Nd:YAG ceramics waveguides,” Opt. Express 21(16), 18963–18968 (2013). 25. S. Y. Choi, T. Calmano, M. H. Kim, D.-I. Yeom, C. Kränkel, G. Huber, and F. Rotermund, “Q-switched operation of a femtosecond-laser-inscribed Yb:YAG channel waveguide laser using carbon nanotubes,” Opt. Express 23(6), 7999–8005 (2015). 26. R. He, J. R. Vázquez de Aldana, and F. Chen, “Passively Q-switched Nd:YVO4 waveguide laser using graphene as a saturable absorber,” Opt. Mater. 46, 414–417 (2015). 27. A. G. Okhrimchuk and P. A. Obraztsov, “11-GHz waveguide Nd:YAG laser CW mode-locked with single-layer graphene,” Sci. Rep. 5(1), 11172 (2015). 28. C. Cheng, H. Liu, Z. Shang, W. Nie, Y. Tan, and J. Blanca del Rosal Rabes, “Vázquez de Aldana, D. Jaque, and F. Chen, “Femtosecond laser written waveguides with MoS2 as saturable absorber for passively Q-switched lasing,” Opt. Mater. Express 6(2), 367–373 (2016). 29. Y. Tan, Z. Guo, L. Ma, H. Zhang, S. Akhmadaliev, S. Zhou, and F. Chen, “Q-switched waveguide laser based on two-dimensional semiconducting materials: tungsten disulfide and black phosphorous,” Opt. Express 24(3), 2858–2866 (2016). 30. C. Cheng, H. Liu, Y. Tan, J. R. Vázquez de Aldana, and F. Chen, “Passively Q-switched waveguide lasers based on two-dimensional transition metal diselenide,” Opt. Express 24(10), 10385–10390 (2016). 31. M. H. Kim, T. Calmano, S. Y. Choi, B. J. Lee, I. H. Baek, K. J. Ahn, D.-I. Yeom, C. Kränkel, and F. Rotermund, “Monolayer graphene coated Yb:YAG channel waveguides for Q-switched laser operation,” Opt. Mater. Express 6(8), 2468–2474 (2016). 32. S. Hakobyan, V. J. Wittwer, K. Hasse, C. Kränkel, T. Südmeyer, and T. Calmano, “Highly efficient Q-switched Yb:YAG channel waveguide laser with 5.6 W of average output power,” Opt. Lett. 41(20), 4715–4718 (2016). 33. W. Nie, R. Li, C. Cheng, Y. Chen, Q. Lu, C. Romero, J. R. Vázquez de Aldana, X. Hao, and F. Chen, “Roomtemperature subnanosecond waveguide lasers in Nd:YVO4 Q-switched by phase-change VO2: A comparison with 2D materials,” Sci. Rep. 7, 46162 (2017). 34. A. G. Okhrimchuk, V. K. Mezentsev, V. V. Dvoyrin, A. S. Kurkov, E. M. Sholokhov, S. K. Turitsyn, A. V. Shestakov, and I. Bennion, “Waveguide-saturable absorber fabricated by femtosecond pulses in YAG:Cr() crystal for Q-switched operation of Yb-fiber laser,” Opt. Lett. 34(24), 3881–3883 (2009).


Introduction
A large variety of photonic systems can now be built in many configurations, being designed to include various compact or miniature laser sources, such as waveguide lasers [1,2].In the past decade a lot of research has been done based on the ability of a femtosecond-(fs-) laser beam to induce controllable changes of the refractive index in an amorphous or crystalline material.Thus, an fs-laser beam was used, for the first time by Davis et al. to inscribe tracks in some glasses [3].In the case of such a material, melting and re-solidification of the irradiated zone provides a line (or a track) with an increased index of refraction compared with that of the medium; consequently, the track itself is used for light propagation.
In another writing technique that is mainly adequate for laser crystals, the fs-laser beam modifies (it can even damage) the crystal inside the irradiated region.Still, an increase of the refractive index is obtained in the adjacent zones by stress field [4].In this case guiding can be realized between two tracks; such a waveguide is suitable for single transverse mode operation, although the narrow distance (of few tens of μm) between the walls imposes limits on the device power scalability.Channel waveguides consisting of two walls have been realized in many laser materials, including Nd:Y 3 Al 5 O 12 (Nd:YAG) [5] and Yb:YAG [6], or Nd:GdVO 4 [7].Efficient laser emission was achieved from such channel waveguides employing as pump source continuous-wave (cw) tunable Ti:sapphire laser.
The buried depressed-cladding waveguide is nowadays recognized as the main configuration that allows power scaling of a waveguide that is directly written by the fs-laser beam technique.In this scheme, many parallel tracks are written around a defined contour [8,9], and a tubular waveguide is obtained by propagating the light inside this structure.Buried depressed-cladding waveguides (of different shapes) were inscribed in Nd:YAG [10] and Nd:YVO 4 [11], Tm:YAG [12] or Pr:YLiF 4 [13] (just to name few of them), from which laser emission performances were evaluated using, mainly, Ti:sapphire laser for the optical pump.Some reviews on the results obtained on various waveguides inscribed by direct writing with fs-laser beam could be found in Ref [2,14,15].Our group have also inscribed circular, buried-depressed cladding waveguide in Nd:YAG and Nd-vanadates, from which watt-level power at 1.06 μm as well as 1.3 μm was obtained in cw regime under the pump with fiber-coupled diode laser [16][17][18].
Cladding waveguides realized by direct writing with an fs-laser beam can be used in other integrated components, such as for beam manipulation [19] or for generation of visible light [20].Very attractive is the possibility to obtain laser pulses with high-peak power by passive Q-switch and to integrate such a laser device for nonlinear conversion applications.For the first time, a circular buried depressed-cladding waveguide (with diameter of 110 μm) was inscribed by Okhrimchuk in a 5.4-mm long diffusion-bonded Nd:YAG/Cr 4+ :YAG composite medium with 57% initial transmission (T 0 ) of Cr 4+ :YAG saturable absorber (SA) [21].The Qswitch operation was investigated in pump-pulse mode with a fiber-coupled diode laser emitting at 808 nm.Laser pulses at 1.06 μm with energy (E p ) of 10 μJ and 1.0-ns duration (t p ) were obtained at 1.0-kHz repetition rate (f p ). Calmano et al. have realized a two-wall channel waveguide in a 1.1-at.%Nd:YAG/Cr 4+ :YAG (T 0 ~30%) composite medium with total length of 9.5 mm [22].The pump with a Ti:sapphire laser enabled Q-switch operation with 300-mW average power (P ave ); the laser pulse energy was E p = 1 μJ at f p = 300 kHz and the shortest pulse duration was t p = 1.0 ns.The same group has realized a similar channel waveguide in Yb:YAG/Cr 4+ :YAG composite medium [23].Passively Q-switch operation with few-ns pulse durations at f p = 600 kHz (P ave = 0.61 W) and E p = 2.7 μJ (peak power, P p around 1 kW) was achieved under the pump at 940 nm with a Ti:sapphire laser.
Other papers reported on laser emission in various waveguides that were inscribed by fslaser beam and that were operated in Q-switch regime with SA media positioned nearby the laser medium.Thus, Q-switch operation of buried depressed double-cladding waveguides that were inscribed in Nd:YAG ceramics was obtained with external semiconductor saturableabsorber mirror (SESAM) [24].Laser pulses with E p ~14 μJ and duration t p = 21 ns at the repetition rate f p = 3.65 MHz were obtained.A channel waveguide that was inscribed in an Yb:YAG crystal was Q-switched by an SA mirror that was made of single-walled carbon nanotubes [25].The laser operated at f p = 1.59 MHz (P ave = 60 mW) with pulses of energy E p = 37.7 nJ and duration t p = 88 ns.A graphene SA mirror was used to passively Q-switch 3D structures that were inscribed in Nd:YAG [19].Average power P ave = 243 mW with pulses at high (above 4 MHz) repetition rate, energy E p ∼55 nJ and duration t p = 70 ns was obtained.A graphene thin film was employed to obtain 1064-nm Q-switch operation from a channel waveguide that was written in Nd:YVO 4 [26].The pulse energy and duration was 8.1 nJ and 25.0 ns, respectively, with an average output power P ave = 129 mW.A single-layer graphene was used to obtain mode-locking in an elliptical buried depressed-cladding waveguide that was inscribed in Nd:YAG; the laser delivered pulses with t p = 16 ps and repetition rate up to f p = 11.3GHz (average power P ave = 12 mW) [27].
Molybdenum disulfide (MoS 2 ) SA film was used for Q-switch operation of a depressedcladding waveguide realized in Nd:YAG crystal [28].Circular depressed-cladding waveguides inscribed in Nd:YAG were operated in Q-switch regime with tungsten disulfide (WS 2 ) and black phosphorous films [29] or WS 2 and molybdenum diselenide membranes that were coated on silica wafers by chemical vapour deposition [30].A monolithic Q-switch waveguide laser was obtained by a monolayer graphene that was transferred onto one end surface of a two-line channel waveguide inscribed in Yb:YAG crystal [31].Apart from other waveguides lasers, in this case the pump was made at 940 nm with a single-mode diode laser.The device delivered laser pulses (at 1029 nm) with energy E p = 64 nJ and duration t p = 96 ns at repetition rate f p = 1.33 MHz (P ave = 85 mW).Recently, high-average power P ave = 5.6 W was reported from an Yb:YAG channel waveguide that was passively Q-switched with an SESAM mirror [32].The laser operated at f p = 5.4 MHz yielding pulses with duration t p = 11 ns and energy E p ∼1 μJ.A VO 2 SA crystal was used to Q-switch superficial cladding waveguides that were inscribed in Nd:YVO 4 [33].Laser pulses with t p = 690 ps were obtained at f p = 2.9 MHz; the average power was P ave = 66.7 mW, indicating that energy E p was around 23 nJ.The depressed-cladding waveguide can be also inscribed in Cr 4+ :YAG SA and then used for passive Q-switching of various configuration, like an Yb-fiber laser [34].
One could observe that most of the works mentioned above have employed as Q-switches SA media that were positioned separately, nearby the waveguide laser.Moreover, very few [21,31] have considered the pump with a diode laser.In addition, the Q-switch with graphene, MOS 2 , WS 2 and black phosphoros films or even SESAM delivered laser pulses with low (few-tens of nJ) energy and limited average output power.Recently, we have reported passive Q-switching with Cr 4+ :YAG SA of a circular buried depressed-cladding waveguide that was inscribed in Nd:YAG ceramics; the pump was done with a fiber-coupled diode laser, but still the SA crystal was positioned nearby the waveguide [17].The laser pulse energy and duration was 19.7 μJ and 2.8 ns, corresponding to a laser peak power of 7 kW.These results show that Cr 4+ :YAG SA is a good choice for obtaining laser pulses at 1.06 μm with both high energy and high peak power, whereas integration as well as the pump with a fiber-coupled diode laser could further increase the interest for such miniature devices.
In this work we report on laser performances obtained from circular, buried depressedcladding waveguides inscribed by fs-laser beam in diffusion-bonded Nd:YAG/Cr 4+ :YAG composite media and that were pumped by a fiber-coupled diode laser.Laser pulses at 1.06 μm with energy E p = 15.7 μJ and duration t p = 3.9 ns at f p = 71.9-kHzrepetition rate were obtained from an waveguide with 150-μm diameter that was realized in a Nd:YAG/Cr 4+ :YAG composite medium that consisted of a 7.0-mm long, 1.0-at.%Nd:YAG crystal and a Cr 4+ :YAG SA crystal with initial transmission T 0 = 0.70.The average output power was P ave = 1.13 W. This seems to be the first demonstration of a circular, buried depressed-cladding waveguide that was inscribed by fs-laser beam in a Nd:YAG/Cr 4+ :YAG composite medium and that was pumped with fiber-coupled diode laser to deliver watt-level average power at 1.06 μm in passive Q-switch regime.

Waveguides fabrication and characterization
In the experiments we used three diffusion-bonded Nd:YAG/Cr 4+ :YAG composite media (Atom Optics Co. Ltd, China).The active side was (in the case of each composite medium) a Nd:YAG crystal with doping level of 1.0-at.%Nd and length of 7.0 mm.The Cr 4+ :YAG SA was also a crystal, with initial transmission (as requested by us and then as specified by the supplier) of T 0 = 0.85 for the first composite medium (denoted by NYAG-1), T 0 = 0.80 for the second composite medium (NYAG-2) and T 0 = 0.70 for the third composite medium (denoted by NYAG-3).The total length of each Nd:YAG/Cr 4+ :YAG composite medium was 8.5 mm for NYAG-1, 9.0 mm for NYAG-2 and 10.3 mm for NYAG-3.
A chirped pulsed amplified system (Clark CPA-2101) that delivered laser pulses at 775 nm with 200-fs duration and energy up to 0.6 mJ, at 2-kHz repetition rate, was used for inscribing the waveguides [16][17][18].A combination of a half-wave plate, a polarizer and calibrated neutral filters was built to control the fs-laser pulse energy (and thus to choose the energy for obtaining tracks in the Nd:YAG/Cr 4+ :YAG composite media).The fs-laser beam was focused with an aspheric lens of 7.5-mm focal length and numerical aperture NA = 0.30; the beam diameter at the focus position was ∼5 μm (in air).The waveguides were realized by the step-by-step writing technique [8,9].Thus, each composite medium was positioned on a motorized XYZ stage that was moved at 100-μm/s speed on Oz direction.Through experiments it was observed that a track can be obtained with fs-laser pulses of 3-μJ energy (measured after the focusing lens).After completing a track, the stage was moved to a different position in the Oxy plane and a new track was inscribed; the distance between two consecutive tracks was set at 5 μm.In this way many parallel tracks were realized around circular contours with defined diameters.The cores with unmodified refractive index are the circular, buried depressed-cladding waveguides; all waveguides were centered 500-μm below the surface of a Nd:YAG/Cr 4+ :YAG composite medium.After inscribing the tracks, the surfaces of each Nd:YAG/Cr 4+ :YAG were polished at laser grade (this reduced the length of both Nd:YAG and Cr 4+ :YAG, but only with few tens of μm).In addition, these sides were coated as antireflection (reflectivity R< 0.25%) at the lasing wavelength λ em = 1.06 μm and with high transmission (transmission T> 0.99) at the pump wavelength λ p = 807 nm.Circular cores with diameter (φ) of 100 μm and 150 μm were obtained in all the Nd:YAG/Cr 4+ :YAG composite media.Results will be presented further for three selected structures.Cross-section views of two circular depressed-cladding waveguides are given in Fig. 1.The waveguide shown in Fig. 1(a) has a diameter φ = 150 μm and it was realized in NYAG-1 (Cr 4+ :YAG with T 0 = 0.85); this waveguide will be denoted by DWG-Q1.A similar waveguide (φ = 150 μm) that was written in the NYAG-3 composite medium (Cr 4+ :YAG with T 0 = 0.70) will be named by DWG-Q3.A microscope view of a circular waveguide with φ = 100 μm (denoted by DWG-Q2) that was obtained in NYAG-2 (Cr 4+ :YAG with T 0 = 0.80) is shown in Fig. 1(b).Guiding in these waveguides is illustrated in Fig. 1(c) and Fig. 1(d) that present views of Cr 4+ :YAG side for DWG-Q1 and DWG-Q2, respectively under the pump at 807 nm.Furthermore, Fig. 1(e) is a photo of the waveguide DWG-Q1 taken from top (in the Oxz plane); the waveguide position is clear and several inscribed tracks can be seen.
In order to evaluate the propagation losses, the light (red at 632.8 nm) of a HeNe laser was coupled (with a coupling efficiency equal to unit) in each waveguide and light power was measured before and after the waveguide.The calculus concluded that the propagation loss at 632.8 nm was 0.9 dB/cm for the waveguide DWG-Q1; also, loss for the waveguide DWG-Q2 and DWG-Q3 amounted to 0.7 dB/cm and 0.6 dB/cm, respectively.Although small, the differences between these losses suggest that improvements of the writing technique are still necessary.On the other hand, these values compares quite well with the losses of 0.8 to 1.4 dB/cm that were reported for various buried depressed-cladding waveguides that were inscribed in Nd:YAG ceramics by the same writing technique [10].Furthermore, loss is decreased in comparison with the values (of up to 1.7 dB/cm) that were measured in our previous work for circular buried depressed-cladding waveguides that were written in Nd:YAG ceramics [17].It should be noted that these losses include some absorption of each Cr 4+ :YAG sample at the 632.8 nm wavelength of the HeNe laser probe.

Laser emission experiments. Results and discussion
The optical pump was made at λ p = 807 nm with a fiber-coupled diode laser (LIMO Co., Germany) that was operated in cw mode.The fiber diameter was 100 μm with numerical aperture NA = 0.22.For collimating the pump beam we used an aspheric lens with focal lens of 50 mm.The focusing was done with an aspheric lens of 40 mm for waveguide DWG-Q2 (φ = 100 μm) whereas in the case of the waveguides with φ = 150 μm a high coupling efficiency (equal to unit) of the pump beam was obtained with an aspheric focusing lens of 60-mm focal length.
Laser emission was achieved in a linear resonator with plane mirrors that were positioned very close of each Nd:YAG/Cr 4+ :YAG composite medium.The resonator rear highreflectivity mirror (HRM) was coated high reflectivity, HR (reflectivity, R> 0.998) at λ em = 1.06 μm and with high transmission (transmission, T> 0.98) at λ p = 807 nm.This mirror was positioned near the Nd:YAG side of a composite medium.The out-coupling mirror (OCM) was placed right after the Cr 4+ :YAG SA; various mirrors with transmission T between 0.05 and 0.60 were used.Each Nd:YAG/Cr 4+ :YAG composite medium was wrapped in Indium foil and fixed in a copper holder whose temperature was maintained at 20°C by a Peltier element.We mention that the pump beam absorption efficiency (η a ) was determined using a 7.0-mm long, 1.0-at.%Nd:YAG crystal (Atom Optics Co. Ltd, China).Measurements concluded that η a ~0.90; therefore, it is considered that the residual pump radiation after Nd:YAG does not affect the initial transmission T 0 of a Cr 4+ :YAG SA crystal.Main parameters of laser emission, like average output power, P ave , pulse repetition rate, f p and pulse duration, t p (FWHM definition) were determined for each waveguide.For example, Fig. 2 presents the dependence of P ave yielded by waveguide DWG-Q1 versus the absorbed pump power, P abs at λ p = 807 nm.One can see that with an OCM of T = 0.10 this waveguide delivered P ave = 0.87 W at λ em = 1.06 μm for P abs = 6.8 W at 807 nm.The repetition rate was f p = 116.9kHz and therefore the laser pulse energy amounted to E p = 7.4 μJ.The pulse duration was t p = 4.2 ns, which indicates a pulse peak power of P p = 1.76 kW.We mention that the laser pulse frequency and duration were measured with a fast UPD-35-IR2-D photodiode (Alphalas, Germany) with a short (<35 ps) rise time and recorded with a Tektronix DPO7254 digital oscilloscope (2.5-GHz bandwidth, 40-GS/s sample rate).On the other hand, when an OCM with T = 0.40 was used, the output power yielded by the waveguide DWG-Q1 increased to P ave = 1.27W. The ratio between P ave and the absorbed pump power P abs was η∼0.19.The repetition rate was f p = 138.8kHz and therefore the pulse energy reached E p = 9.15 μJ.The laser pulse peak power was P p = 1.99 kW.The absorbed pump power at threshold was P abs ~1.0 W for the OCM with T = 0.10 and it increased to P abs ~1.5 W for the OCM with T = 0.40.The best performances obtained from all three waveguides are plotted in Fig. 3 for an OCM with transmission T = 0.40.The waveguide DWG-Q3 (that was written in NYAG-3, the composite medium with Cr 4+ :YAG of T 0 = 0.70) yielded an average power P ave = 1.13 W at P abs = 6.8 W [Fig. 3(a)].The repetition rate varied linearly with P abs [as shown in Fig. 3(b)], increasing from f p = 12.3 kHz at low levels (P ave = 0.16 W, P abs ∼2.0 W) up to f p = 71.9kHz

Fig. 3 .
Fig. 3. Characteristics of Q-switch operation obtained from all circular, buried depressedcladding waveguides, OCM with T = 0.40.(a) Average output power, P ave .The laser pulse temporal shape and the laser beam near-field distribution are shown at the indicated point.(b) Laser pulse repetition rate.(c) Laser pulse energy, E p and corresponding peak power, P p .